溶解度表
镧、锂、硫、镥、铝

| 物质 | 化学式 | 0 °C | 10 °C | 20 °C | 30 °C | 40 °C | 50 °C | 60 °C | 70 °C | 80 °C | 90 °C | 100 °C |
| --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- |
| 乙酸镧 | La(C2H3O2)3·H2O |  |  | 16.9 |  |  |  |  |  |  |  |  |
| 溴酸镧 | La(BrO3)3 | 98 | 120 | 149 | 200 |  |  |  |  |  |  |  |
| 碘酸镧 | La(IO3)3 |  |  | 4.575×10−2 |  |  |  |  |  |  |  |  |
| 钼酸镧 | La2(MoO4)3 |  |  | 2.473×10−3 |  |  |  |  |  |  |  |  |
| 硝酸镧 | La(NO3)3 | 100 |  | 136 |  | 168 |  | 247 |  |  |  |  |
| 硒酸镧 | La2(SeO4)3 | 50.5 | 45 | 45 | 45 | 45 |  | 18.5 |  | 5.4 | 2.2 |  |
| 硫酸镧 | La2(SO4)3 | 3 | 2.72 | 2.33 | 1.9 | 1.67 |  | 1.26 |  | 0.91 | 0.79 | 0.68 |
| 钨酸镧 | La2(WO4)3·3H2O |  |  | 6.06 |  |  |  |  |  |  |  |  |
| 乙酸锂 | LiC2H3O2 | 31.2 | 35.1 | 40.8 | 50.6 | 68.6 |  |  |  |  |  |  |
| 叠氮化锂 | LiN3 | 61.3 | 64.2 | 67.2 | 71.2 | 75.4 |  | 86.6 |  |  |  | 100 |
| 苯甲酸锂 | LiC7H5O2 | 38.9 | 41.6 | 44.7 | 53.8 |  |  |  |  |  |  |  |
| 溴酸锂 | LiBrO3 | 154 | 166 | 179 | 198 | 221 |  | 269 |  | 308 | 329 | 355 |
| 溴化锂 | LiBr | 143 | 147 | 160 | 183 | 211 |  | 223 |  | 245 |  | 266 |
| 碳酸锂 | Li2CO3 | 1.54 | 1.43 | 1.33 | 1.26 | 1.17 | 1.08 | 1.01 |  | 0.85 |  | 0.72 |
| 氯酸锂 | LiClO3 | 241 | 283 | 372 | 488 | 604 |  | 777 |  |  |  |  |
| 氯化锂 | LiCl | 69.2 | 74.5 | 83.5 | 86.2 | 89.8 |  | 98.4 |  | 112 | 121 | 128 |
| 铬酸锂 | Li2CrO4.2H2O |  |  | 142 |  |  |  |  |  |  |  |  |
| 重铬酸锂 | Li2Cr2O7.2H2O |  |  |  | 151 |  |  |  |  |  |  |  |
| 磷酸二氢锂 | LiH2PO4 | 126 |  |  |  |  |  |  |  |  |  |  |
| 氟化锂 | LiF |  |  | 0.16 |  |  |  |  |  |  |  |  |
| 氟硅酸锂 | Li2SiF6.2H2O |  |  | 73 |  |  |  |  |  |  |  |  |
| 甲酸锂 | LiHCO2 | 32.3 | 35.7 | 39.3 | 44.1 | 49.5 |  | 64.7 |  | 92.7 | 116 | 138 |
| 亚磷酸氢锂 | Li2HPO3 | 4.43 |  |  | 9.97 | 7.61 |  | 7.11 |  |  |  | 6.03 |
| 氢氧化锂 | LiOH | 12.7 | 12.7 | 12.8 | 12.9 | 13.0 | 13.3 | 13.8 |  | 15.3 |  | 17.5 |
| 碘化锂 | LiI | 151 | 157 | 165 | 171 | 179 |  | 202 |  | 435 | 440 | 481 |
| 钼酸锂 | Li2MoO4 | 82.6 |  | 79.5 | 79.5 | 78 |  |  |  |  |  | 73.9 |
| 硝酸锂 | LiNO3 | 53.4 | 60.8 | 70.1 | 138 | 152 |  | 175 |  |  |  |  |
| 亚硝酸锂 | LiNO2 | 70.9 | 82.5 | 96.8 | 114 | 133 |  | 177 |  | 233 | 272 | 324 |
| 草酸锂 | Li2C2O4 |  |  | 8 |  |  |  |  |  |  |  |  |
| 高氯酸锂 | LiClO4 | 42.7 | 49 | 56.1 | 63.6 | 72.3 |  | 92.3 |  | 128 | 151 |  |
| 高锰酸锂 | LiMnO4 |  |  | 71.4 |  |  |  |  |  |  |  |  |
| 磷酸锂 | Li3PO4 |  |  | 0.039 |  |  |  |  |  |  |  |  |
| 硒化鋰 | Li2Se |  |  | 57.7 |  |  |  |  |  |  |  |  |
| 亚硒酸锂 | Li2SeO3 | 25 | 23.3 | 21.5 | 19.6 | 17.9 |  | 14.7 |  | 11.9 | 11.1 | 9.9 |
| 硫酸锂 | Li2SO4 | 36.1 | 35.5 | 34.8 | 34.2 | 33.7 |  | 32.6 |  | 31.4 | 30.9 |  |
| 酒石酸锂 | Li2C4H4O6 | 42 | 31.8 | 27.1 | 26.6 | 27.2 |  | 29.5 |  |  |  |  |
| 硫氰酸锂 | LiSCN |  |  | 114 | 131 | 153 |  |  |  |  |  |  |
| 钒酸锂 | LiVO3 | 2.5 |  | 4.82 | 6.28 | 4.38 |  | 2.67 |  |  |  |  |
| 二氧化硫 | SO2 | 22 | 15 | 11 | 8 | 6.5 | 5 | 4 | 3.5 | 3.4 | 3.5 | 3.7 |
| 氢氧化镥 | Lu(OH)3 |  |  | 1.164×10−5 |  |  |  |  |  |  |  |  |
| 硫酸镥 | Lu2(SO4)3·8H2O |  |  | 57.9 |  |  |  |  |  |  |  |  |
| 氯化铝 | AlCl3 | 44.9 | 46.3 |  | 47.0 |  |  | 46.5 |  |  |  |  |
| 氯化铝，六水 | AlCl3·6H2O | 43.9 | 44.9 | 45.8 | 46.6 | 47.3 |  | 48.1 |  | 48.6 |  | 49 |
| 氟化铝 | AlF3 | 0.56 | 0.56 | 0.67 | 0.78 | 0.91 |  | 1.1 |  | 1.32 |  | 1.72 |
| 硝酸铝 | Al(NO3)3 | 60 | 66.7 | 73.9 | 81.8 | 88.7 |  | 106 |  | 132 | 153 | 160 |
| 高氯酸铝 | Al(ClO4)3 | 122 | 128 | 133 |  |  |  |  |  |  |  |  |
| 硫酸铝 | Al2(SO4)3 | 31.2 | 33.5 | 36.4 | 40.4 | 45.8 |  | 59.2 |  | 73 | 80.8 | 89 |
| 氢氧化铝 | Al(OH)3 |  |  | 0.0001 |  |  |  |  |  |  |  |  |